LMucko/crystallography-open-database huggingface dataset:
The crystal structures of Na4 Fe (C N)6 (H2 O)10 and Na4 Mn (C N)6 (H2 O)10
Tullberg, A.; Vannerberg, N.G.; Acta Chemica Scandinavica (1-27,1973-42,1988) 25 (1971) 343–344; doi:

data_1528155
_publ_section_title
;
 The crystal structures of Na4 Fe (C N)6 (H2 O)10 and Na4 Mn (C N)6 (H2
 O)10
;
_journal_name_full
'Acta Chemica Scandinavica (1-27,1973-42,1988)'
_journal_page_first              343
_journal_page_last               344
_journal_volume                  25
_journal_year                    1971
_chemical_formula_sum            'C6 H20 Mn N6 Na4 O10'
_chemical_name_systematic        'Na4 Mn (C N)6 (H2 O)10'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_cell_angle_alpha                90
_cell_angle_beta                 97.5
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   9.8
_cell_length_b                   11.4
_cell_length_c                   9
_cell_volume                     996.878
_citation_journal_id_ASTM        ACSAA4
_cod_data_source_file            Tullberg_ACSAA4_1971_1190.cif
_cod_data_source_block           C6H20Mn1N6Na4O10
_cod_original_sg_symbol_Hall     '-P 2ybc (x-z,y,z)'
_cod_original_formula_sum        'C6 H20 Mn1 N6 Na4 O10'
_cod_database_code               1528155
The crystal structure of Na2 Fe (C N)5 N H3 (H2 O)2
Tullberg, A.; Vannerberg, N.G.; Acta Chemica Scandinavica (1-27,1973-42,1988) 26 (1972) 3382–3383; doi:

data_1528156
_publ_section_title
;
 The crystal structure of Na2 Fe (C N)5 N H3 (H2 O)2
;
_journal_name_full
'Acta Chemica Scandinavica (1-27,1973-42,1988)'
_journal_page_first              3382
_journal_page_last               3383
_journal_volume                  26
_journal_year                    1972
_chemical_formula_sum            'C5 H7 Fe N6 Na2 O2'
_chemical_name_systematic        'Na2 Fe (C N)5 N H3 (H2 O)2'
_space_group_IT_number           58
_symmetry_space_group_name_Hall  '-P 2 2n'
_symmetry_space_group_name_H-M   'P n n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   6.1
_cell_length_b                   11.9
_cell_length_c                   15.5
_cell_volume                     1125.145
_citation_journal_id_ASTM        ACSAA4
_cod_data_source_file            Tullberg_ACSAA4_1972_1213.cif
_cod_data_source_block           C5H7Fe1N6Na2O2
_cod_original_formula_sum        'C5 H7 Fe1 N6 Na2 O2'
_cod_database_code               1528156
The crystal structure of aluminium hydride
Turley, J.W.; Rinn, H.W.; Inorganic Chemistry 8 (1969) 17–22; doi:

data_4343801
_publ_section_title
;
 The crystal structure of aluminium hydride
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              17
_journal_page_last               22
_journal_volume                  8
_journal_year                    1969
_chemical_formula_sum            'Al H3'
_space_group_IT_number           167
_symmetry_space_group_name_Hall  '-R 3 2"c'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            6
_cell_length_a                   4.4493
_cell_length_b                   4.4493
_cell_length_c                   11.8037
_cell_volume                     202.363
_citation_journal_id_ASTM        INOCAJ
_cod_data_source_file            Turley_INOCAJ_1969_1314.cif
_cod_data_source_block           H3Al1
_cod_original_cell_volume        202.3635
_cod_original_formula_sum        'H3 Al1'
_cod_database_code               4343801
The crystal structure of aluminium hydride
Turley, J.W.; Rinn, H.W.; Inorganic Chemistry 8 (1969) 17–22; doi:

data_4343802
_publ_section_title
;
 The crystal structure of aluminium hydride
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              17
_journal_page_last               22
_journal_volume                  8
_journal_year                    1969
_chemical_formula_sum            'Al D3'
_space_group_IT_number           167
_symmetry_space_group_name_Hall  '-R 3 2"c'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            6
_cell_length_a                   4.4309
_cell_length_b                   4.4309
_cell_length_c                   11.7744
_cell_volume                     200.195
_citation_journal_id_ASTM        INOCAJ
_cod_data_source_file            Turley_INOCAJ_1969_1315.cif
_cod_data_source_block           D3Al1
_cod_original_formula_sum        'D3 Al1'
_cod_database_code               4343802
Synthesis and X-ray diffraction study of single crystals of a new pyrochlore containing lithium, Sr Li Ta2 O6 F
Tutov, A.G.; Bader, V.I.; Myl'nikova, I.E.; Kristallografiya 17 (1972) 406–407; doi:

data_1528157
_publ_section_title
;
 Synthesis and X-ray diffraction study of single crystals of a new
 pyrochlore containing lithium, Sr Li Ta2 O6 F
;
_journal_name_full               Kristallografiya
_journal_page_first              406
_journal_page_last               407
_journal_volume                  17
_journal_year                    1972
_chemical_formula_sum            'F Li O6 Sr Ta2'
_chemical_name_systematic        'Sr Li Ta2 O6 F'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  'F 4d 2 3 -1d'
_symmetry_space_group_name_H-M   'F d -3 m :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   10.47
_cell_length_b                   10.47
_cell_length_c                   10.47
_cell_volume                     1147.731
_citation_journal_id_ASTM        KRISAJ
_cod_data_source_file            Tutov_KRISAJ_1972_1898.cif
_cod_data_source_block           F1Li1O6Sr1Ta2
_cod_original_sg_symbol_Hall     '-F 4vw 2vw 3 (x+1/8,y+1/8,z+1/8)'
_cod_original_formula_sum        'F1 Li1 O6 Sr1 Ta2'
_cod_database_code               1528157
The crystal structure of basic tellurium nitrate, Te2 O4 (H N O3)
Twink, L.N.; Carpenter, G.B.; Acta Crystallographica (1,1948-23,1967) 21 (1966) 578–583; doi:

data_2310502
_publ_section_title
;
 The crystal structure of basic tellurium nitrate, Te2 O4 (H N O3)
;
_journal_name_full               'Acta Crystallographica (1,1948-23,1967)'
_journal_page_first              578
_journal_page_last               583
_journal_volume                  21
_journal_year                    1966
_chemical_formula_sum            'H N O7 Te2'
_chemical_name_systematic        '(Te2 O4) (H N O3)'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   14.547
_cell_length_b                   8.77
_cell_length_c                   4.446
_cell_volume                     567.208
_citation_journal_id_ASTM        ACCRA9
_cod_data_source_file            Twink_ACCRA9_1966_1065.cif
_cod_data_source_block           H1N1O7Te2
_cod_original_cell_volume        567.2083
_cod_original_formula_sum        'H1 N1 O7 Te2'
_cod_database_code               2310502
An X-ray examination of the indium-rich alloys of the systems In-Pb and In-Hg
Tyzack, C.; Raynor, G.V.; Rossteutscher, W.; Transactions of the Faraday Society 50 (1954) 675–684; doi:

data_1528158
_publ_section_title
;
 An X-ray examination of the indium-rich alloys of the systems In-Pb and
 In-Hg
;
_journal_name_full               'Transactions of the Faraday Society'
_journal_page_first              675
_journal_page_last               684
_journal_volume                  50
_journal_year                    1954
_chemical_formula_sum            'Hg0.055 In0.945'
_chemical_name_systematic        '(Hg0.055 In0.945)'
_space_group_IT_number           139
_symmetry_space_group_name_Hall  '-I 4 2'
_symmetry_space_group_name_H-M   'I 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   3.2693
_cell_length_b                   3.2693
_cell_length_c                   4.8586
_cell_volume                     51.930
_citation_journal_id_ASTM        TFSOA4
_cod_data_source_file            Tyzack_TFSOA4_1954_547.cif
_cod_data_source_block           Hg0.055In0.945
_cod_original_cell_volume        51.93029
_cod_database_code               1528158
Electron diffraction study of the structure of ammonium sulfate
Udalova, V.V.; Pinsker, Z.G.; Kristallografiya 8 (1963) 538–547; doi:

data_1528159
_publ_section_title
;
 Electron diffraction study of the structure of ammonium sulfate
;
_journal_name_full               Kristallografiya
_journal_page_first              538
_journal_page_last               547
_journal_volume                  8
_journal_year                    1963
_chemical_formula_sum            'H8 N2 O4 S'
_chemical_name_systematic        '(N H4)2 (S O4)'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2n 2a'
_symmetry_space_group_name_H-M   'P m c n'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.97
_cell_length_b                   10.6
_cell_length_c                   7.76
_cell_volume                     491.068
_citation_journal_id_ASTM        KRISAJ
_cod_data_source_file            Udalova_KRISAJ_1963_1684.cif
_cod_data_source_block           H8N2O4S1
_cod_original_cell_volume        491.0683
_cod_original_sg_symbol_Hall     '-P 2ac 2n (y,z,x)'
_cod_original_formula_sum        'H8 N2 O4 S1'
_cod_database_code               1528159
Crystal Structure of Thorium Nitrate Pentahydrate by X-ray Diffraction
Ueki, T.; Zalkin, A.; Templeton, D.H.; Acta Crystallographica (1,1948-23,1967) 20 (1966) 836–841; doi:

data_2310503
_publ_section_title
;
 Crystal Structure of Thorium Nitrate Pentahydrate by X-ray Diffraction
;
_journal_name_full               'Acta Crystallographica (1,1948-23,1967)'
_journal_page_first              836
_journal_page_last               841
_journal_volume                  20
_journal_year                    1966
_chemical_formula_sum            'H10 N4 O17 Th'
_chemical_name_systematic        'Th (N O3)4 (H2 O)5'
_space_group_IT_number           43
_symmetry_space_group_name_Hall  'F 2 -2d'
_symmetry_space_group_name_H-M   'F d d 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   11.182
_cell_length_b                   22.873
_cell_length_c                   10.573
_cell_volume                     2704.213
_citation_journal_id_ASTM        ACCRA9
_cod_data_source_file            Ueki_ACCRA9_1966_1094.cif
_cod_data_source_block           H10N4O17Th1
_cod_original_formula_sum        'H10 N4 O17 Th1'
_cod_database_code               2310503
Triammonium scandium selenate
Valkonen, J.; Niinisto, L.; Acta Crystallographica B (24,1968-38,1982) 34 (1978) 266–268; doi:

data_2106456
_publ_section_title
;
 Triammonium scandium selenate
;
_journal_name_full               'Acta Crystallographica B (24,1968-38,1982)'
_journal_page_first              266
_journal_page_last               268
_journal_volume                  34
_journal_year                    1978
_chemical_formula_sum            'H12 N3 O12 Sc Se3'
_chemical_name_systematic        '(N H4)3 Sc (Se O4)3'
_space_group_IT_number           146
_symmetry_space_group_name_Hall  'R 3'
_symmetry_space_group_name_H-M   'R 3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            6
_cell_length_a                   15.567
_cell_length_b                   15.567
_cell_length_c                   9.871
_cell_volume                     2071.580
_citation_journal_id_ASTM        ACBCAR
_cod_data_source_file            Valkonen_ACBCAR_1978_826.cif
_cod_data_source_block           H12N3O12Sc1Se3
_cod_original_cell_volume        2071.58
_cod_original_formula_sum        'H12 N3 O12 Sc1 Se3'
_cod_database_code               2106456
New ternary gallides with the K Hg2 and Ca In2 structures
Vasilechko, L.O.; Grin', Yu.; Fedorchuk, A.A.; Neorganicheskie Materialy 30 (1994) 1409–1411; doi:

data_1528160
_publ_section_title
;
 New ternary gallides with the K Hg2 and Ca In2 structures
;
_journal_name_full               'Neorganicheskie Materialy'
_journal_page_first              1409
_journal_page_last               1411
_journal_volume                  30
_journal_year                    1994
_chemical_formula_sum            'Ga1.2 Ni0.8 Y'
_chemical_name_systematic        '(Ga0.6 Ni0.4)2 Y'
_space_group_IT_number           74
_symmetry_space_group_name_Hall  '-I 2b 2'
_symmetry_space_group_name_H-M   'I m m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   4.304
_cell_length_b                   6.99
_cell_length_c                   7.431
_cell_volume                     223.561
_citation_journal_id_ASTM        NMATEI
_cod_data_source_file            Vasilechko_NMATEI_1994_522.cif
_cod_data_source_block           Ga1.2Ni0.8Y1
_cod_original_cell_volume        223.5613
_cod_original_formula_sum        'Ga1.2 Ni0.8 Y1'
_cod_database_code               1528160
New ternary gallides with the K Hg2 and Ca In2 structures
Vasilechko, L.O.; Grin', Yu.; Fedorchuk, A.A.; Neorganicheskie Materialy 30 (1994) 1409–1411; doi:

data_1528161
_publ_section_title
;
 New ternary gallides with the K Hg2 and Ca In2 structures
;
_journal_name_full               'Neorganicheskie Materialy'
_journal_page_first              1409
_journal_page_last               1411
_journal_volume                  30
_journal_year                    1994
_chemical_formula_sum            'Ga1.6 Ni0.4 Y'
_chemical_name_systematic        '(Ga0.8 Ni0.2)2 Y'
_space_group_IT_number           194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   4.342
_cell_length_b                   4.342
_cell_length_c                   7.249
_cell_volume                     118.355
_citation_journal_id_ASTM        NMATEI
_cod_data_source_file            Vasilechko_NMATEI_1994_523.cif
_cod_data_source_block           Ga1.6Ni0.4Y1
_cod_original_cell_volume        118.3555
_cod_original_formula_sum        'Ga1.6 Ni0.4 Y1'
_cod_database_code               1528161
Synthesis, structure, and properies of a new intermetallic compound, Ca7 Ni4 Sn13
Vennos, D.A.; DiSalvo, F.J.; Badding, M.E.; Journal of the Less-Common Metals 175 (1991) 339–346; doi:

data_1528162
_publ_section_title
;
 Synthesis, structure, and properies of a new intermetallic compound, Ca7
 Ni4 Sn13
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              339
_journal_page_last               346
_journal_volume                  175
_journal_year                    1991
_chemical_formula_sum            'Ca7 Ni4 Sn13'
_space_group_IT_number           83
_symmetry_space_group_name_Hall  '-P 4'
_symmetry_space_group_name_H-M   'P 4/m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   11.2
_cell_length_b                   11.2
_cell_length_c                   4.594
_cell_volume                     576.271
_citation_journal_id_ASTM        JCOMAH
_cod_data_source_file            Vennos_JCOMAH_1991_252.cif
_cod_data_source_block           Ca7Ni4Sn13
_cod_original_cell_volume        576.2713
_cod_database_code               1528162
New A-15 phases
Vielhaber, E.; Luo, H.L.; Solid State Communications 5 (1967) 221–223; doi:

data_1528163
_publ_section_title
;
 New A-15 phases
;
_journal_name_full               'Solid State Communications'
_journal_page_first              221
_journal_page_last               223
_journal_volume                  5
_journal_year                    1967
_chemical_formula_sum            'Ti3.2 Tl0.8'
_chemical_name_systematic        'Ti3 (Ti0.2 Tl0.8)'
_space_group_IT_number           223
_symmetry_space_group_name_Hall  '-P 4n 2 3'
_symmetry_space_group_name_H-M   'P m -3 n'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.256
_cell_length_b                   5.256
_cell_length_c                   5.256
_cell_volume                     145.200
_citation_journal_id_ASTM        SSCOA4
_cod_data_source_file            Vielhaber_SSCOA4_1967_128.cif
_cod_data_source_block           Ti3.2Tl0.8
_cod_original_cell_volume        145.1998
_cod_database_code               1528163
Ueber Oxocadmate: K2 Cd2 O3
Vielhaber, E.; Hoppe, R.; Zeitschrift fuer Anorganische und Allgemeine Chemie 382 (1971) 270–280; doi:

data_1528164
_publ_section_title
;
 Ueber Oxocadmate: K2 Cd2 O3
;
_journal_name_full
'Zeitschrift fuer Anorganische und Allgemeine Chemie'
_journal_page_first              270
_journal_page_last               280
_journal_volume                  382
_journal_year                    1971
_chemical_formula_sum            'Cd2 K2 O3'
_chemical_name_systematic        'K2 Cd2 O3'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 116
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   6.417
_cell_length_b                   6.723
_cell_length_c                   6.586
_cell_volume                     255.374
_citation_journal_id_ASTM        ZAACAB
_cod_data_source_file            Vielhaber_ZAACAB_1971_1919.cif
_cod_data_source_block           Cd2K2O3
_cod_original_cell_volume        255.3742
_cod_database_code               1528164
Note on the crystal structure of vanadium dichloride
Villadsen, J.; Acta Chemica Scandinavica (1-27,1973-42,1988) 13 (1959) 2146–2146; doi:

data_1528165
_publ_section_title
;
 Note on the crystal structure of vanadium dichloride
;
_journal_name_full
'Acta Chemica Scandinavica (1-27,1973-42,1988)'
_journal_page_first              2146
_journal_page_last               2146
_journal_volume                  13
_journal_year                    1959
_chemical_formula_sum            'Cl2 V'
_chemical_name_systematic        'V Cl2'
_space_group_IT_number           164
_symmetry_space_group_name_Hall  '-P 3 2"'
_symmetry_space_group_name_H-M   'P -3 m 1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   3.6
_cell_length_b                   3.6
_cell_length_c                   5.83
_cell_volume                     65.434
_citation_journal_id_ASTM        ACSAA4
_cod_data_source_file            Villadsen_ACSAA4_1959_1729.cif
_cod_data_source_block           Cl2V1
_cod_original_cell_volume        65.4341
_cod_original_formula_sum        'Cl2 V1'
_cod_database_code               1528165
The Crystal Structure of Lithium Hydroxylammonium Sulphate
Vilminot, S.; Anderson, M.R.; Brown, I.D.; Acta Crystallographica B (24,1968-38,1982) 29 (1973) 2628–2630; doi:

data_2106457
_publ_section_title
;
 The Crystal Structure of Lithium Hydroxylammonium Sulphate
;
_journal_name_full               'Acta Crystallographica B (24,1968-38,1982)'
_journal_page_first              2628
_journal_page_last               2630
_journal_volume                  29
_journal_year                    1973
_chemical_formula_sum            'H4 Li N O5 S'
_chemical_name_systematic        'Li N H3 O H S O4'
_space_group_IT_number           61
_symmetry_space_group_name_Hall  '-P 2ac 2ab'
_symmetry_space_group_name_H-M   'P b c a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   18.46
_cell_length_b                   7.28
_cell_length_c                   6.712
_cell_volume                     902.018
_citation_journal_id_ASTM        ACBCAR
_cod_data_source_file            Vilminot_ACBCAR_1973_1037.cif
_cod_data_source_block           H4Li1N1O5S1
_cod_original_cell_volume        902.0176
_cod_original_formula_sum        'H4 Li1 N1 O5 S1'
_cod_database_code               2106457
Environnement de l'etain(II) dans les fluorohalogenures: etude de Sn3 Br F5
Vilminot, S.; Granier, W.; le Cot, L.; Acta Crystallographica B (24,1968-38,1982) 34 (1978) 35–37; doi:

data_2106458
_publ_section_title
;
 Environnement de l'etain(II) dans les fluorohalogenures: etude de Sn3 Br
 F5
;
_journal_name_full               'Acta Crystallographica B (24,1968-38,1982)'
_journal_page_first              35
_journal_page_last               37
_journal_volume                  34
_journal_year                    1978
_chemical_formula_sum            'Br F5 Sn3'
_chemical_name_systematic        'Sn3 Br F5'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_cell_angle_alpha                90
_cell_angle_beta                 90.36
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   4.295
_cell_length_b                   12.639
_cell_length_c                   12.784
_cell_volume                     693.959
_citation_journal_id_ASTM        ACBCAR
_cod_data_source_file            Vilminot_ACBCAR_1978_815.cif
_cod_data_source_block           Br1F5Sn3
_cod_original_cell_volume        693.9595
_cod_original_sg_symbol_Hall     '-P 2ybc (x-z,y,z)'
_cod_original_formula_sum        'Br1 F5 Sn3'
_cod_database_code               2106458
The anti-Th3 P4 - type structure in the lanthanum - rhodium system: La4 Rhca3.0
Virkar, A.V.; Yingh, P.P.; Raman, A.; Inorganic Chemistry 9 (1970) 353–356; doi:

data_4343803
_publ_section_title
;
 The anti-Th3 P4 - type structure in the lanthanum - rhodium system: La4
 Rhca3.0
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              353
_journal_page_last               356
_journal_volume                  9
_journal_year                    1970
_chemical_formula_sum            'La4 Rh2.91'
_space_group_IT_number           220
_symmetry_space_group_name_Hall  'I -4bd 2c 3'
_symmetry_space_group_name_H-M   'I -4 3 d'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   8.922
_cell_length_b                   8.922
_cell_length_c                   8.922
_cell_volume                     710.210
_citation_journal_id_ASTM        INOCAJ
_cod_data_source_file            Virkar_INOCAJ_1970_1813.cif
_cod_data_source_block           La4Rh2.91
_cod_original_cell_volume        710.2098
_cod_database_code               4343803